Chapter Outline. Diffusion  how do atoms move through solids?


 Adela Jenkins
 2 years ago
 Views:
Transcription
1 Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law) NonsteadyState iffusion (Fick s second law) Factors that influence diffusion iffusing species Host solid Temperature Microstructure
2 What is diffusion? iffusion is material transport by atomic motion. results of an atomistic simulation of atomic mixing homework project in MSE 4592/6270 Inhomogeneous materials can become homogeneous by diffusion. For an active diffusion to occur, the temperature should be high enough to overcome energy barriers to atomic motion. 2
3 Interdiffusion and Selfdiffusion Interdiffusion (or impurity diffusion) occurs in response to a concentration gradient. (Heat) Before After Selfdiffusion is diffusion in onecomponent material, when all atoms that exchange positions are of the same type. 3
4 iffusion Mechanisms (I) Vacancy diffusion mechanism Atom migration Vacancy migration Before After To jump from lattice site to lattice site, atoms need energy to break bonds with neighbors, and to cause the necessary lattice distortions during jump. This energy comes from the thermal energy of atomic vibrations (E av ~ k B T) The direction of flow of atoms is opposite the vacancy flow direction. 4
5 iffusion Mechanisms (II) Interstitial diffusion mechanism Interstitial atom before jump Interstitial atom after jump Interstitial diffusion is generally faster than vacancy diffusion because bonding of interstitials to the surrounding atoms is normally weaker and there are many more interstitial sites than vacancy sites to jump to. Requires small impurity atoms (e.g. C, H, O) to fit into interstices in host. 5
6 iffusion Flux The flux of diffusing atoms, J, is used to quantify how fast diffusion occurs. The flux is defined as either the number of atoms diffusing through unit area per unit time (atoms/m 2 second) or the mass of atoms diffusing through unit area per unit time, (kg/m 2  second). For example, for the mass flux we can write J M / At (/A) (dm/dt) (Kg m 2 s  ) where M is the mass of atoms diffusing through the area A during time t. A J 6
7 SteadyState iffusion Steady state diffusion: the diffusion flux does not change with time. Concentration profile: concentration of atoms/molecules of interest as function of position in the sample. Concentration gradient: dc/dx (Kg m 4 ): the slope at a particular point on concentration profile. dc dx ΔC Δx C x A A C x B B 7
8 Fick s first law: the diffusion flux along direction x is proportional to the concentration gradient J SteadyState iffusion: Fick s first law dc dx where is the diffusion coefficient The concentration gradient is often called the driving force in diffusion (but it is not a force in the mechanistic sense). The minus sign in the equation means that diffusion is down the concentration gradient. 8
9 iffusion down the concentration gradient J dc dx Why do the random jumps of atoms result in a flux of atoms from regions of high concentration towards the regions of low concentration? Atoms here jump randomly both right and left But there are not many atoms here to jump to the left As a result there is a net flux of atoms from left to right. 9
10 NonsteadyState iffusion: Fick s second law In many real situations the concentration profile and the concentration gradient are changing with time. The changes of the concentration profile can be described in this case by a differential equation, Fick s second law. C t x C x 2 C 2 x Solution of this equation is concentration profile as function of time, C(x,t): 0
11 NonsteadyState iffusion: Fick s second law C t 2 C 2 x Fick s second law relates the rate of change of composition with time to the curvature of the concentration profile: C C C x x x Concentration increases with time in those parts of the system where concentration profile has a positive curvature. And decreases where curvature is negative. The phenomenological description based on the Fick s laws is valid for any atomic mechanism of diffusion. Understanding of the atomic mechanisms is important, however, for predicting the dependence of the atomic mobility (and, therefore, diffusion coefficient) on the type of interatomic bonding, temperature, and microstructure.
12 iffusion Thermally Activated Process (I) (not tested) To jump from lattice site to lattice site, atoms need energy to break bonds with neighbors, and to cause the necessary lattice distortions during jump. The energy necessary for motion, E m, is called the activation energy for vacancy motion. Energy Atom E m Vacancy istance Schematic representation of the diffusion of an atom from its original position into a vacant lattice site. Activation energy E m has to be supplied to the atom so that it could break interatomic bonds and to move into the new position. 2
13 iffusion Thermally Activated Process (II) (not tested) The average thermal energy of an atom (k B T ev for room temperature) is usually much smaller that the activation energy E m (~ ev/atom) and a large fluctuation in energy (when the energy is pooled together in a small volume) is needed for a jump. The probability of such fluctuation or frequency of jumps, R j, depends exponentially on temperature and can be described by equation that is attributed to Swedish chemist Arrhenius: R j R exp E m 0 k BT where R 0 is socalled attempt frequency proportional to the frequency of atomic vibrations. 3
14 iffusion Thermally Activated Process (III) (not tested) For the vacancy diffusion mechanism the probability for any atom in a solid to move is the product of the probability of finding a vacancy in an adjacent lattice site (see Chapter 4): Q P z exp v kbt R j R exp E m 0 k BT The diffusion coefficient can be estimated as z is coordination number (number of atoms adjacent to the vacancy) and the frequency of jumps (probability of thermal fluctuation needed to overcome the energy barrier for vacancy motion): zr 0 0 a 2 E exp m k B T ( E Q ) + exp m V Q exp k B T V k 0 B T exp Q d k B T Temperature dependence of the diffusion coefficient, follows the Arrhenius dependence. 4
15 iffusion Temperature ependence (I) J dc dx iffusion coefficient is the measure of mobility of diffusing species. Q exp d 0 RT 0 temperatureindependent preexponential (m 2 /s) Q d the activation energy for diffusion (J/mol or ev/atom) R the gas constant (8.3 J/molK or ev/atomk) T absolute temperature (K) The above equation can be rewritten as ln Qd ln0 R T log Qd or log0 2.3R T The activation energy Q d and preexponential 0, therefore, can be estimated by plotting ln versus /T or log versus /T. Such plots are called Arrhenius plots. 5
16 iffusion Temperature ependence (II) b log 0 y ax+ b a Qd 2.3R x /T Graph of log vs. /T has slop of Q d /2.3R, intercept of log o log log 0 Qd 2.3R T Q d log 2.3R T log T 2 2 6
17 Temperature dependence: Interstitial and vacancy diffusion mechanisms (I) log log0 Q d 2.3R T iffusion of interstitials is typically faster as compared to the vacancy diffusion mechanism (selfdiffusion or diffusion of substitutional atoms). 7
18 Temperature dependence: Interstitial and vacancy diffusion mechanisms Q d 0exp k BT Impurity 0, mm 2 /s  Q d, kj/mol Interstitial diffusion mechanism C in FCC Fe C in BCC Fe N in FCC Fe N in BCC Fe H in FCC Fe H in BCC Fe Smaller atoms cause less distortion of the lattice during migration and diffuse more readily than big ones (the atomic diameters decrease from C to N to H). iffusion is faster in open lattices or in open directions Vacancy diffusion mechanism Fe in FCC Fe Fe in BCC Fe Ni in Cu Si in Si 0, mm 2 /s Q d, kj/mol
19 Example: Temperature dependence of At 300ºC the diffusion coefficient and activation energy for Cu in Si are (300ºC) 7.8 x 0  m 2 /s Q d 4.5 kj/mol What is the diffusion coefficient at 350ºC? transform data ln Temp T /T Q d 0 ln ln0 R T Q d exp k BT ln 2 ln 0 Q R d T2 and ln ln 0 Q R d T ln 2 ln ln 2 Q R d T2 T 9
20 Example: Temperature dependence of (continued) ln Q R T2 T 2 d 2 exp Q R d T2 T T K T K 2 (7.8 x 0 m 2 /s) 4,500 J/mol exp 8.34 J/mol  K 623 K 573 K x 0  m 2 /s 20
21 iffusion: Role of the microstructure (I) Selfdiffusion coefficients for Ag depend on the diffusion path. In general the diffusivity if greater through less restrictive structural regions grain boundaries, dislocation cores, external surfaces. 2
22 iffusion: Role of the microstructure (II) The plots below are from the computer simulation by T. Kwok, P. S. Ho, and S. Yip. Initial atomic positions are shown by the circles, trajectories of atoms are shown by lines. We can see the difference between atomic mobility in the bulk crystal and in the grain boundary region. 22
23 Example: iffusion in nanocrystalline materials Lin et al. J. Phys. Chem. C 4, 5686, 200 Arrhenius plots for 59 Fe diffusivities in nanocrystalline Fe and other alloys compared to the crystalline Fe (ferrite). [Wurschum et al. Adv. Eng. Mat. 5, 365, 2003] 23
24 Factors that influence diffusion: Summary Temperature  diffusion rate increases very rapidly with increasing temperature iffusion mechanism diffusion by interstitial mechanism is usually faster than by vacancy mechanism iffusing and host species  o, Q d are different for every solute, solvent pair Microstructure  diffusion is faster in polycrystalline materials compared to single crystals because of the accelerated diffusion along grain boundaries. 24
25 iffusion in material processing Case Hardening: Hardening the surface of a metal by exposing it to impurities that diffuse into the surface region and increase surface hardness. Common example of case hardening is carburization of steel. iffusion of carbon atoms (interstitial mechanism) increases concentration of C atoms and makes iron (steel) harder. oping silicon with phosphorus for ntype semiconductors. Process of doping:. eposit P rich layers on surface. silicon 2. Heat it. 3. Result: oped semiconductor regions. silicon 25
26 Summary Make sure you understand language and concepts: Activation energy Concentration gradient iffusion iffusion coefficient iffusion flux riving force Fick s first and second laws Interdiffusion Interstitial diffusion Selfdiffusion Steadystate diffusion Nonsteadystate diffusion Temperature dependence of Vacancy diffusion 26
27 Homework #3: 5.7, 5.8, 5.22, 5.23, 5.2 ue date: Monday, September 20. Reading for next class: Chapter 6: Mechanical Properties of Metals Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic eformation Yield Strength Tensile Strength uctility Resilience Toughness Hardness Optional reading (not tested): details of the different types of hardness tests, variability of material properties (starting from the middle of page 74) 27
Introduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationSurface Treatments. Corrosion Protective coatings for harsh environments (catalytic converters, electrochemical cells )
Surface Treatments Applications Biomedical (biocompatible coatings on implants, drug coatings for sustained release ) Mechanical Tribological friction and wear (tool steels, implants ) Fatigue minimize
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationCrystal Defects p. 2. Point Defects: Vacancies. Department of Materials Science and Engineering University of Virginia. Lecturer: Leonid V.
Crystal Defects p. 1 A twodimensional representation of a perfect single crystal with regular arrangement of atoms. But nothing is perfect, and structures of real materials can be better represented by
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationCHAPTER 6: DIFFUSION IN SOLIDS. Interdiffusion. Simple Diffusion. Diffusion Steady and NonSteady State ISSUES TO ADDRESS...
CHAPTER 6: DIFFUSION IN SOLIDS Diffusion Steady and NonSteady State ISSUES TO ADDRESS... Gear from casehardened steel (C diffusion) Diffusion  Mass transport by atomic motion How does diffusion occur?
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationAerogel an excellent thermal insulator (known as frozen smoke)
Aerogel an excellent thermal insulator (known as frozen smoke) 2 Thermal images of a dog (top) and a snake wrapped around a human arm (bottom) Thermal Properties (1) Heat Capacity Heat Capacity When heated,
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationMaterial Strengthening Mechanisms. Academic Resource Center
Material Strengthening Mechanisms Academic Resource Center Agenda Definition of strengthening Strengthening mechanisms Grain size reduction Solid solution alloying Cold Working (strain hardening) Three
More informationVysoká škola báňská Technická univerzita Ostrava. Physical Metallurgy. Didactic Text. Jaroslav Sojka
Vysoká škola báňská Technická univerzita Ostrava Physical Metallurgy Didactic Text Jaroslav Sojka Ostrava 2013 Physical Metallurgy Review: Prof. Ing. Ludmila Hypecká, DrSc. Description: Physical Metallurgy
More informationConstitutive Equations  Plasticity
MCEN 5023/ASEN 5012 Chapter 9 Constitutive Equations  Plasticity Fall, 2006 1 Mechanical Properties of Materials: Modulus of Elasticity Tensile strength Yield Strength Compressive strength Hardness Impact
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationRef. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield
MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Nibase superalloys.
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationMechanisms of Diffusion in Materials 3.205 L4 11/7/06
Mechanisms of Diffusion in Materials 1 A final point on interdiffusion The composition profiles resulting from interdiffusion are generally constrained by phase equilibria. Consider the an Ir Re diffusion
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More information in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons
Free Electrons in a Metal  in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons  if these electrons would behave like an ideal gas
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationBasic laws and electrical properties of metals (I) Electrical properties. Basic laws and electrical properties of metals (II)
Electrical properties Electrical conduction How many moveable electrons are there in a material (carrier density)? How easily do they move (mobility)? Semiconductivity Electrons and holes Intrinsic and
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationChapter 3: Kinetics of Electrode Reactions
Goal: To understand the observed behavior of electrode kinetics with respect to potential and concentration. = i/nfa (mol/scm 2 ) Rate = f(e) Dynamic Equilibrium A k f k b B s 1 f = k f C A (M/s) b =
More informationLecture Outline Real Structure
Lecture Outline Real Structure Point Defects (zerodimensional) they move by diffusion Line defects Dislocations, onedimensional they move by glide Observing Dislocations Significance of Dislocations
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationCHAPTER 7: DISLOCATIONS AND STRENGTHENING
CHAPTER 7: DISLOCATIONS AND STRENGTHENING ISSUES TO ADDRESS... Why are dislocations observed primarily in metals and alloys? Mech 221  Notes 7 1 DISLOCATION MOTION Produces plastic deformation, in crystalline
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationLecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationDO PHYSICS ONLINE. conduction band. ~ 6 ev. Fig. 1. Energy band diagram for diamond (insulator) and silicon (semiconductor).
DO PHYSIS ONLINE FROM IDEAS TO IMPLEMENTATION 9.4.3 ATOMS TO TRANSISTORS SEMIONDUTORS ENERGY BANDS Diamond is a very good insulator. The electronic configuration in the ground state is 1s 2 2s 2 2. It
More informationKinetic Monte Carlo: from transition probabilities to transition rates
Kinetic Monte Carlo: from transition probabilities to transition rates With MD we can only reproduce the dynamics of the system for 100 ns. Slow thermallyactivated processes, such as diffusion, cannot
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationLayer Deposition: Thermal Oxidation and CVD. Rupesh Gupta IIT Delhi Supervisor: Dr. Chacko Jacob
1 Layer Deposition: Thermal Oxidation and CVD Rupesh Gupta IIT Delhi Supervisor: Dr. Chacko Jacob 2 OUTLINE Thermal Oxidation and Model o Factors Affecting Kinetics o Future Trends: Oxidation o CVD and
More informationChapter 14 Chemical Kinetics
Chapter 14 Chemical Kinetics Chemical kinetics: the area of chemistry dealing with the speeds or rates at which reactions occur. Rates are affected by several factors: The concentrations of the reactants:
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationEnergy of a Dislocation
Energy of a Dislocation The Line Tension T Broken and stretched bonds around the dislocation There is EXTRA energy associated with the Defect T = G 2 r 2 b J m G = Shear Modulus Total Extra Energy in the
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationLecture 34 Kinetics Topics: Effect of Temperature, Collision Theory, Activated Complex Theory. Chapter
34.1 5.111 Lecture 34 Kinetics Topics: Effect of Temperature, Collision Theory, Activated Complex Theory. Chapter 13.1113.13 Effect of Temperature on Reaction Rates GasPhase A qualitative observation
More information[ A] 2. [ A] 2 = 2k dt. [ A] o
Chemistry 360 Dr Jean M Standard Problem Set 3 Solutions The reaction 2A " P follows secondorder kinetics The rate constant for the reaction is k350 0 4 Lmol s Determine the time required for the concentration
More informationSolid State Detectors = SemiConductor based Detectors
Solid State Detectors = SemiConductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the pn junction Charge collection
More informationDefinition : Characteristics of Metals :
Metallic Bond Definition : It may be defined as, 1. The force that binds a metal ion to a number of electrons with in its sphere of influence. 2. The attractive force which holds the atoms of two or more
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationELECTRONIC DEVICES MENJANA MINDA KREATIF DAN INOVATIF
INTRODUCTION TO ELECTRONIC DEVICES MENJANA MINDA KREATIF DAN INOVATIF Introduction What is Electronics? Electronic Devices? Electronic Systems? introduction Electronics: The branch of physics that deals
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationCHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS
191 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of
More informationKINETIC MOLECULAR THEORY OF MATTER
KINETIC MOLECULAR THEORY OF MATTER The kineticmolecular theory is based on the idea that particles of matter are always in motion. The theory can be used to explain the properties of solids, liquids,
More informationStrengthening. Mechanisms of strengthening in singlephase metals: grainsize reduction solidsolution alloying strain hardening
Strengthening The ability of a metal to deform depends on the ability of dislocations to move Restricting dislocation motion makes the material stronger Mechanisms of strengthening in singlephase metals:
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More information3. Diodes and Diode Circuits. 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1
3. Diodes and Diode Circuits 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1 3.1 Diode Characteristics SmallSignal Diodes Diode: a semiconductor device, which conduct the current
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationMartensite in Steels
Materials Science & Metallurgy http://www.msm.cam.ac.uk/phasetrans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used
More informationThe MaxwellBoltzmann Distribution
The MaxwellBoltzmann Distribution Gases are composed of atoms or molecules. These atoms or molecules do not really interact with each other except through collisions. In many cases, we may think of a
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More information5.6 Isobaric thermal expansion and isothermal compression (Hiroshi Matsuoka)
5.6 Isobaric thermal expansion and isothermal compression Hiroshi Matsuoka 1 5.6.2 he coefficient of thermal expansion as a response function to a temperature change he coefficient of thermal expansion
More informationMaterial Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India
Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 5612 India Chapter 15. Thermal properties Engineering materials are important
More informationProcessing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur
Processing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur Lecture  8 Diffusion and Ion Implantation II (Refer
More informationTHERMAL PROPERTIES. How do ceramics, metals, and polymers rank? M. Medraj / PM WoodAdams Mech. Eng. Dept.  Concordia University MECH 221 Fall 2008/1
THERMAL PROPERTIES How does a material respond to heat? How do we define and measure...  heat capacity  coefficient of thermal expansion  thermal conductivity  thermal shock resistance How do ceramics,
More informationORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS
ORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS K. Sztwiertnia Polish Academy of Sciences, Institute of Metallurgy and Materials Science, 25 Reymonta St., 30059 Krakow, Poland MMN 2009
More informationSemiconductors, diodes, transistors
Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!
More informationStates of Matter CHAPTER 10 REVIEW SECTION 1. Name Date Class. Answer the following questions in the space provided.
CHAPTER 10 REVIEW States of Matter SECTION 1 SHORT ANSWER Answer the following questions in the space provided. 1. Identify whether the descriptions below describe an ideal gas or a real gas. ideal gas
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationInrush Current Limiters
Inrush Current Limiters General technical information Date: May 2009 EPCOS AG 2009. Reproduction, publication and dissemination of this publication, enclosures hereto and the information contained therein
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationThis is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th
More informationModule #17. Work/Strain Hardening. READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter
Module #17 Work/Strain Hardening READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter D. KuhlmannWilsdorf, Trans. AIME, v. 224 (1962) pp. 10471061 Work Hardening RECALL: During plastic deformation,
More informationSize effects. Lecture 6 OUTLINE
Size effects 1 MTX9100 Nanomaterials Lecture 6 OUTLINE Why does size influence the material s properties? How does size influence the material s performance? Why are properties of nanoscale objects
More information